Table of Contents Introduction .............................................................................................................................................................. 2 Chemistry .............................................................................................................................................................. 2-4 Industrial Formulators’ Epoxies ................................................................................................................. 4-5 Safety and Handling ............................................................................................................................................ 5 Measuring and Mixing Epoxy Systems ................................................................................................. 6-7 Techniques of Epoxy Use .............................................................................................................................. 7-8 Coating with Epoxy Resin ............................................................................................................................ 8-9 Fiberglassing with Epoxy Resin ............................................................................................................. 9-11 Using Fillers with Epoxy Resins .......................................................................................................... 12-13 Epoxy Resins as Strustural Adhesives ............................................................................................. 13-14 Filleting, Fairing and Molding with Epoxy Resins ..................................................................... 15-16 Painting and Finishing ............................................................................................................................. 16-17 Troubleshooting ................................................................................................................................................... 17
about the use of these products as outlined in this booklet is a distillation of the knowledge we have gained over the years. This is to help you, the user, to be in charge. Your responsibility is to make sure that all the products you use, including ours, are used properly. The section on chemistry may seem a bit of a mystery to some of you, but a rudimentary understanding will help you complete your tasks more efficiently.
When you begin to work with epoxy resins, it’s always useful to know a little of their history. The dictionary defines epoxy as “heat setting resin made by the chemical bonding of smaller molecules into larger ones.” While that may be over simplifying things a little, in all epoxies, that is basically what is happening. What becomes complicated is the thousands of variations that make each chemical compound used in the manufacture of epoxy resin formulations specifically different to perform the job it was designed to do.
You’ll find here sections on basic chemistry and safety regarding all epoxies. Proper measuring and mixing techniques are next. And we finish with a useful section on troubleshooting.
Scientists have been aware of epoxy resins for many years but the first commercial exploration of their properties was undertaken in the 1930’s. This was in Germany by the firm of I.G. Farben Industries. However, it was not until the 1950’s that use of the compounds in a commercial way was introduced in North America. At about this time the founder of Industrial Formulators, Jim Peters B.Sc., began experimenting with them and over the years became one of the leading formulators in the world.
A thorough knowledge of epoxy resin chemistry is not necessary before you start, but having a basic chemical knowledge will help you complete your project more effectively. The resin that is the basis for most of our epoxy formulations is the diglycidol ether of bisphenol A (DGEBA). Bisphenol A is produced by reacting phenol with acetone under suitable conditions. Bis means two, phenyl means phenol groups and the “A” stands for acetone. Thus, bisphenol A is the chemical product made from chemically combining two phenols with one acetone. Unreacted acetone and phenol are stripped from the bisphenol A which is then reacted with a material called epichlorohydrin. This reaction sticks the two (di) glycidyl groups on ends of the bisphenol A molecule. The resultant product is the diglycidyl ether of bisphenyl A, or the basic epoxy resin. It is these glycidyl groups that react with the amine hydrogen atoms on hardeners to produce the cured epoxy resin.
Epoxies are among the “thermoset” family of resins, along with polyester, silicones, urethanes, melamines, acrylics and phenolics. Once curing of epoxies has taken place they cannot be melted by heat. This makes epoxies the opposite of such other plastics (thermoplastics) like polyethylene, vinyl, polypropylene, etc., which can be melted and solidified over and over again. Industrial Formulators, Inc. supplies epoxies for industries such as construction, electronics, marine, automotive, sporting goods and hobbies. Our epoxy formulations have been used to solve problems and are used regularly in pulp mills, submarines, dams, museums, railroads and research labs along with more standard uses like boat building and electrical potting. We are experimenting with new uses for epoxy resins all the time.
Basic epoxy resin is very viscous and unsuitable for use except as a thick glue for specialized applications. At Industrial Formulators Inc., we purchase the material in this basic form, then modify it using formulae developed by us. The result is the various epoxy resin systems we offer.
Our responsibility is to provide quality products to our customers. The information
Hardeners used with room temperature cured epoxy resins are most commonly polyamines. That is, they are organic molecules containing two or more amine groups. Amine groups are not unlike ammonia in structure except that they are attached to organic molecules. Like ammonia, amines are strongly alkaline. Because of this similarity, epoxy resin hardeners often have an ammonialike odor, most notable in the dead air space in containers right after they are opened. Once in the open this odor is difficult to detect because of the low vapor pressure of the polyamines.
that can accommodate one, or by changing the temperature and mass of the resin/ hardener mix. The epoxy curing reaction is exothermic. This means that it gives off heat as it cures. The rate at which the epoxy resin cures is dependent upon the curing temperature. The warmer it is the faster it goes. The curing rate will vary by about half or double with each 10°C (18°F) change in temperature. For example, if an epoxy system takes 3 hours to become tack free at 21°C (70°F), it will be tack free in 1.5 hours at 31°C (88°F) or tack free in 6 hours at 11°C (52F). Everything to do with the speed of the reaction follows this general rule. Pot life and working time are greatly influenced by the initial temperature of the mixed resin and hardener.
Reactive amine groups are nitrogen atoms with one or two hydrogen atoms attached to the nitrogen. These hydrogen atoms react with oxygen atoms from glycidol groups on the epoxy to form the cured resin - a highly crosslinked thermoset plastic. Heat will soften, but not melt a cured epoxy. The three-dimensional structure gives the cured resin excellent physical properties.
The gel time of the resin is the time it takes for a given mass held in a compact volume to solidify. Gel time depends on the initial temperature of the mass and follows the above rule. Cure time is surface area/mass sensitive in addition to being temperature sensitive.
The ratio of the glycidol oxygens to the amine hydrogens, taking into account the various molecular weights and densities involved, determines the final resin to hardener ratio. Varying the recommended ratio will leave either unreacted oxygen or hydrogen atoms depending upon which side is in excess. The resultant cured resin will have lower strength, as it is not as completely crosslinked.
What’s happening is this: as the reaction proceeds it gives off heat. If the heat generated is immediately dissipated to the environment (as occurs in thin films) the temperature of the curing resin does not rise and the reaction speed proceeds at a uniform pace. If the resin is confined (as in a mixing pot) the exothermic reaction raises the temperature of the mixture, accelerating the reaction.
Epoxy hardeners are not catalysts. Catalysts promote reactions but do not chemically become a part of the finished product. Epoxy hardeners mate with the epoxy resin, greatly contributing to the ultimate properties of the cured system.
Working time is about 75% of the gel time for the size and shape of the pot. It can be lengthened by increasing the surface area or working with a smaller batch. Material left in the pot will increase in absolute viscosity measured at 24°C (75°F), for example, due to polymerization but initially decrease in apparent viscosity due to heating. Material left in the pot to 75% of gel time may appear quite thin (due to heating) but will actually be quite thick when cooled to room temperature. Thick, partially cured epoxy is not as effective in wetting out fiberglass cloth and bonding surfaces. Experienced users either mix batches that
Cure time of an epoxy system is dependent upon the reactivity of the amine hydrogen atoms. While the attached organic molecule takes no direct part in the chemical reaction, it does influence how readily the amine hydrogen atoms leave the nitrogen and react with the glycidol oxygen atom. Thus, cure time is set by the kinetics of the particular amine used in the hardener. Cure time can be altered only by selecting a different hardener, adding an accelerator in systems
will be applied almost immediately or increase the surface area to slow the reaction, thus increasing working time.
exposure will induce chalking and eventually the epoxy will disintegrate, losing its mechanical properties. The solution to this problem is to protect the epoxy coating with paint or with a varnish which contains an ultraviolet light shield.
Although the cure rate of an epoxy is dependent upon temperature, the curing mechanism is independent of temperature. The reaction proceeds most quickly in the liquid state. As the cure proceeds the system changes from a liquid to a sticky viscous soft gel. After gelation the reaction speed slows down as hardness increases. Chemical reactions proceed more slowly in the solid state. From the soft sticky gel the system gets harder, slowly losing its stickiness. It becomes tack free and continues to become harder and stronger as time passes.
Caution must be observed when using epoxy resins along with polyester resins. Observe the general rule that epoxy resins may be applied over cured polyesters that have been dewaxed and well-sanded but polyesters should never be used over cured epoxy resins. Unreacted amine in the epoxy inhibits the peroxide catalyst in the polyester causing an incomplete cure at the interface. Sanding does not get rid of the unreacted amine. The result is a poor bond even though the surface appears cured. Debonding will be the inevitable result.
At normal temperatures the system will reach about 60 to 80% of ultimate strength after 24 hours. Curing then proceeds slowly over the next several weeks, finally reaching a point where no further curing will occur without a significant increase in temperature. However, for most purposes, room temperature cured systems can be considered fully cured after 72 hours at 25°C (77°F).
Industrial Formulators’ Epoxies
A surface film may form in some epoxy systems during the curing process. Technically, this surface film is an amine carbamate that can form in the presence of carbon dioxide and water vapor. More appears on cool damp days than on warm sunny days. This film is water-soluble and should be removed with soap and water before sanding and re-coating or painting. This occurs mainly when using 51-Cure or Cold Cure with Jet Cure Hardener. All epoxies should be sanded lightly but thoroughly before recoating, or recoated within 72 hours.
Industrial Formulators’ epoxies are formulated systems, meaning that we start with basic epoxy resins manufactured by large chemical companies and modify them to make them suitable for the required end use. In the first modification (for most products) we reduce the viscosity by the addition of diluents or low viscosity solvents, which are also epoxies. This makes an epoxy system thin enough to wet fiberglass cloth, coat wood and bind various fillers to produce gap filling glues and putties. Because the diluents we use are also epoxies, they are called reactive diluents, reacting with the amines the same way the basic resin reacts, becoming a part of the cured system. Other materials protect against long term embrittlement and improve resiliency and impact resistance. Finally, trace materials designed to lower surface tension, promote substrate wet out, reduce cratering and “fisheye” formation, aid in breaking bubbles and detraining air are used to produce the finished product.
Unprotected exterior epoxy resin coatings are not ultimately sunlight resistant. After about six months of exposure to intense sunlight they begin to degrade. Additional
These modifications are what make our epoxy systems unique and different from others. We develop the chemical formulations for our epoxy resins and hardeners. To ensure our
It is usually more efficient to work with as fast a cure time as practical for the application at hand. This allows the builder to get along to the next phase without wasting time waiting for epoxy to cure. Faster curing films with shorter tack times will have less chance to pick up fly tracks, bugs, and other airborne contaminants.
Keep Epoxy Resins and Hardeners off your skin Wear disposable gloves or barrier skin creams (available from Industrial Formulators Inc.) when working with epoxy resins. Never use solvents to remove epoxies from your skin. Solvents, in addition to having problems that are as bad or worse than epoxies, can help drive the hazardous ingredients into your body. If accidental contact occurs, use a good handsoap and lots of water and paper towels to remove epoxy from your skin. Then apply a good medicated skin cream to replace the natural oils removed by the handsoap. Using a solvent to remove partially cured epoxy from your body is not an acceptable alternative.
desired level of quality, all of our epoxy products are produced in our manufacturing facility. Every batch gets tested for both gel time and “thin film set time”. Nothing is shipped to a customer that does not meet our high standards. Everything we ship cures if properly measured and thoroughly mixed. The diverse background of our staff gives us the unique advantage of knowing and applying epoxy technology far better than others in the business. The development, manufacture, and distribution of Industrial Formulators products is our only business, and our staff takes pride in being personally available to all of our customers.
If a rash develops when working with epoxies you should stop until it clears up. If the rash is bad or persists see a doctor. Take him a copy of this book and have him contact us if he needs additional information. Don’t continue to work with epoxy if you break out every time you get near it. This is your body’s way of telling you to cool it. Pay attention.
The dominant factor in the design, development, and evolution of Industrial Formulators products has been this:
An Epoxy System should adapt to the conditions of the user - Not the other way around.
Safety and Handling
Working cleanly and keeping epoxy off you are the keystones of epoxy safety. Work in a throwaway mode. Don’t try to clean brushes with solvent - toss them out. Tools like putty knives can be wiped with a paper towel then sanded clean after the epoxy cures. Cured epoxy doesn’t stick to polyethylene or wax paper. Gloves, disposable brushes, and one time use roller covers are expendable. Your health is not. Think of gloves and dust masks as another part of the cost of the project, being prepared to spend some money on these items designed to help protect you. We like the inexpensive disposable gloves as opposed to heavier, more permanent gloves. The problem with the heavier gloves is that they eventually become contaminated with uncured resin or hardener on the inside long before they wear out. The very thing that you started using to protect you is now a source of contamination. Disposable gloves wear out about the time they become dirty and are replaced.
We select our resin and hardener raw materials with the health and safety of our customers in mind. However, it is not possible to make a hazard-free epoxy resin system. As with all chemical products, they must be handled properly to minimize health risks. Material Safety Data Sheets (MSDS) are available upon request for all of our products. The primary hazard when working with an epoxy system is skin irritation leading to possible skin sensitization from prolonged and repeated direct skin contact. Most people who become sensitized are unable to continue working with epoxies without breaking out in a rash commonly on the inside of the forearms and on the forehead above the eyebrows. The effect appears to be cumulative. That is, you might be able to get away with getting epoxy on your skin for awhile but sooner or later it can catch up to you and you will be sensitized. We would like to emphasize that these products can be used safely for a lifetime – if handled properly.
The vapor pressure of epoxy resins and hardeners is so low that vapors rarely cause problems, unless you have already become sensitized. Well-cured resin should cause no problem, as it is largely inert.
Develop a measuring technique that is sufficiently accurate and then stay with it. Doing it the same way each time will minimize the chance for error. In the interest of simplification the following discussion assumes a 2:1 volume ratio. Refer to our catalog for specific product mix ratios.
Whenever sanding or creating any kind of dust wear a mask along with safety glasses and gloves to keep the dust out of your lungs. If you sand fiberglass and allow the dust to get on your skin you will probably get an itch from the glass fibers. Shower in cool water to wash the fibers off you. The itch usually goes away after 24 hours.
If you are using some type of graduated cup or a straight-sided can, get in the habit of measuring the same way each time. If you pour the resin first, then always pour the resin first. Before you add the hardener, notice how much resin is already in the container, divide this by two (for a 2:1 system) and then add hardener to bring the total to the correct mark. Measuring in the same order each time will avoid the common error of two parts of hardener to one part of resin.
Epoxy resins and hardeners have a low flammability risk generally burning only if exposed to a high heat source. BUT, the solvents found in S-1 and Titanium are flammable, and vapors can even be explosive in the right concentration. Be smart and avoid any possible source of ignition when using solvents.
Using a vertically held stir stick marked in a two to one ratio will only work for vertical sided containers. Don’t use this method on containers with sloping sides.
Most people never develop health problems working with epoxy resins. If we scared you a little then it’s our hope that you’ll work with these materials a little smarter and cleaner than you might have otherwise.
If you use the “two measures/one measure” method and mix in a separate pot, be sure to scrape the sides each time you pour from your measuring cups to the mixing pot.
Measuring and Mixing Epoxy Systems
Make sure the graduations on disposable cups look right. Some paper cups are not rolled correctly when made – the first graduation sometimes is too high or too low. We can’t inspect each cup to make sure it was properly made – this is your job.
Measuring and mixing is really easy because most of our epoxy systems mix at a 1:1 or 2:1 volume ratio. This doesn’t mean you don’t have to pay attention to what you’re doing. Occasionally a customer will call suggesting that something is wrong with the epoxy because it didn’t cure properly. We know of no situation where the resin/ hardener has gone bad or has been contaminated and wouldn’t cure. It always resolves that the batch was either improperly measured or insufficiently mixed in the user’s shop. Epoxy chemistry just will not allow it to work any other way.
For small batches less than 90 ml (3 oz.) use the syringes or accumeasure kit. Industrial Formulators Inc. offers one mechanical pump for those who desire the convenience that is devices provides. These pumps are the kind that you find at the ballpark and use to get mustard out of the jar to put on your hot dog. Complete instructions come with each plunger pump kit. We recommend using the pumps to dispense, not measure. Pump into a graduated mixing cup or tub to be double sure of an accurate measure.
Measuring errors are insidious and can pop up when you least expect them. These errors usually occur because you changed your technique, were in a hurry, had someone else mix a batch, or were just not careful.
Be aware that any mechanical device can go haywire, lying to you with a straight face. Valves can stick causing backflow into the reservoirs. Cool temperatures can cause the viscosity to change. The rate or speed that you pump can alter delivery volumes.
Techniques of Epoxy Use Four epoxy application techniques are commonly used. These are coating, fiberglassing, gluing and filleting/fairing. Furthermore, the techniques are pretty much the same whether they are involved in wood or fiberglass construction and repair. After all, coating with epoxy involves the same technique and tools regardless of whether the substrate is wood, fiberglass, or something else.
Epoxy systems can be measured by weight as well as volume. The correct ratios vary so if you plan to mix by weight give our technical support line a call. Don’t make the mistake of using the volume ratio when measuring by weight. The hardener is less dense than the resin you’ll use too much hardener and get an incomplete cure.
What might seem to be other techniques are usually just variations or combinations of the above. Many of our epoxy users discover new variations. We will discuss a number of these variations and the “tricks” that will make the epoxy work go easier and faster. We don’t know everything and are constantly learning something new. We invite you to learn along with us.
Large batches (a litre or more) are most efficiently measured by weight. A postal scale is usually accurate enough for the larger batches. An O’Haus triple beam balance will allow for the accurate weighing of batches from as little as a few grams to over 2.5 kilograms.
If you come up with a variation that we don’t mention, model it first to see if it will work. Do this prior to using the whole project as a test. For example, we are often asked if Cold Cure epoxy will stick to stained wood. Most of the time it will if stain used is water or alcohol based. However, the only way to be really sure is to conduct your own little test.
With the resin and hardener accurately measured, mix thoroughly. Stir well, scraping the container sides, and mix from the bottom to the top. Keep stirring until that mixture is no longer hazy. Don’t worry about a few air bubbles. That’s normal. Scrape the mixing stick several times on the side of the container Don’t make large batches. Keep in mind that large batches take longer to mix, have a much shorter pot life, and if you get side tracked cost more when they gel in the pot. Epoxy paperweights are expensive.
Suppose that you are staining a piece of fir that will later be coated with epoxy and have another piece laminated to it. First, stain a scrap piece of the same wood; allow it to dry well (several days). Laminate on two pieces of 3 or 4 inch wide fiberglass tape about fifteen cm long. Leave a “tail” that can be grasped later with a pair of pliers by running the tape about half way up on a plastic squeegee. Let the epoxy cure a day or two. Remove the squeegee and grab the tail with the pliers. Try to peel the tape off the substrate. If the tape tears where the tail starts leaving the balance of the tape bonded to the surface, then the bond is good. If the whole thing pops off intact then the bond is bad and the stain is interfering with the bond strength. Better find a new stain and repeat the test.
If you measured or mixed incorrectly and a batch doesn’t properly cure about the only thing to do is scrape it off and start over. A hot air gun will help to soften the partially cured material. Then try removing any residual with acetone, MEK, or lacquer thinner (but not with the hot air gun or source of ignition around). Wear solvent resistant gloves and have plenty of ventilation when doing this. Then examine your technique to find out what went wrong.
This same procedure can be modified to test the ability of the epoxy to bond exotic woods. If the failure occurs in the wood when two
pieces are glued rather than in the glue line then it is safe to assume that the epoxy works on that kind of wood.
pull away from the surface creating craters. Overheating will also cause the expansion of any air in the pores of the wood and may result in an epoxy coating full of bubbles.
In order to simplify the following discussion of the four main areas of use for our epoxy systems we are going to confine the discussion to using Cold Cure epoxy with plywood, a common building material. Where appropriate we will mention the use of our other epoxy systems. The sections following this will discuss modifications of the four techniques for specific areas of building and repairing fiberglass structures. We feel that if you can understand and use the following techniques then you will be able to skillfully do most kinds of epoxy work.
Sometimes a coating will try to crater. This is most common with coatings that are too thin, recoated surfaces that have not been thoroughly sanded or on contaminated surfaces but may happen on other surfaces as well. While the cause of cratering is quite complex, the solution is pretty simple. Immediately after coating a surface look at it from an angle, sweeping your eyes over the whole surface. Craters will usually form within ten minutes after first applying the coating. If cratering occurs, take the heel of the foam roller and really grind it in the area that has cratered. This wets out the dry spots in the crater center. Then, re-roll the area treated to even out the coating.
Coating with Epoxy Resin Whenever possible it is best to do coating operations on the bench. If the part is too large or cumbersome to place on the bench, then whenever possible arrange your work so that it is horizontal. When working flat you’re not fighting gravity and the coated panel is easily sanded on the bench using a disc sander and foam pad. Coating a sheet of fir plywood will illustrate this method.
Cold Cure epoxy will bond and cure in thin coatings in cold, damp conditions without any special tricks, but giving it an induction period will help speed things along. After mixing the resin and hardener allow the mix to sit in the pot for 15 to 20 minutes. Then apply it in the usual manner. The use of a hot air gun will help level a cold epoxy coating but it is not necessary to aid in the cure.
Mix the resin and hardener in the correct ratio. Pour this mix on the plywood in a stream of “S” curves starting at one end and finishing at the other, making four or five curves along the length. Spread the epoxy back and forth with a squeegee into the dry areas, trying to get as even a coating as possible without being too fussy. Use a dry foam roller to even out the coating. When this first coat is cured to at least a soft set tack free stage it can be recoated.
After 24 to 48 hours (depending upon temperature and hardener used) the coating will be cured enough to sand. First wipe the surface with a damp sponge to remove any water soluble amine carbamate surface film prior to sanding (for Jet Cure or 51-Cure only). At this stage of cure the epoxy coating can usually be sanded with a disc sander and a big foam pad starting with 60 grit paper. Disk sanding can generate quite a bit of heat, especially when the sandpaper gets dull or clogged, causing gumming of the sanding disk. Keep the sander moving and apply only light pressure. This keeps the heat down. If clogging still happens you’ll have to either hand sand, scrape as described below, wet sand or allow another day for the cure to proceed.
Use at least two coats for interior wood and three in areas that may be constantly wet. Several tricks can be used to improve the appearance of the finished film. Bubbles that persist in the coating can be broken with a foam brush by lightly dragging it across the surface. Fanning the uncured surface with a hot air gun or hair dryer will accomplish this with greater speed. Avoid overheating an area as this could cause the epoxy film to
Scraping is an alternative to sanding that actually produces a better finish. This shaves off a thin film of epoxy leaving a surface that looks like it was sanded with 600 grit paper.
Small parts can be scraped using a single edged razor held vertically. Several companies make wood scrapers for working on larger surfaces. Keep them sharp and be careful not to cut yourself.
more coats of varnish and is much more durable. Revarnishing is much easier because the old varnish is just removed down to the epoxy coating. Epoxy coatings should be sanded before varnishing or painting. These materials stick to the epoxy by mechanical means and must have some “tooth” in order to bond well.
Sanding dust should be removed by blowing or brushing it off prior to recoating. The final bit may be removed with a damp rag. Don’t use acetone, or other solvents. Tack rags may leave an unbondable surface coating on the sanded epoxy surface.
Fiberglassing with Epoxy Resin
Some amine cured epoxy surfaces are quite alkaline and can react with any acidic material such as moist carbon dioxide or silicates. Further epoxy coats may not bond well to some of these reaction products. Sanding, in addition to providing some “tooth” for mechanical bonding, also cleans since it exposes new, uncontaminated surface. If in doubt, sand.
Exterior surfaces usually use fiberglass or other woven cloth material as a reinforcement, or substrate, allowing a thicker, stronger epoxy coating which results in higher abrasion, impact and moisture resistance. In the case of most wood composite structures, the purpose of this reinforcing cloth is to strengthen the epoxy coating, not to reinforce the part.
Try to work at a constant or falling temperature when coating. When the temperature is rising, air trapped beneath the uncured epoxy may expand and cause small bubbles to form in the coating. Avoid working in direct sunlight for this reason. If you must work in sunlight, do your coating as the sun is going down. The surface will be cooling and air bubbles should not form. Evening dew condensation does not harm the partially cured Cold Cure epoxy coating.
Cold Cure epoxy is a much better choice over wood than polyester resin. Polyester is a poor adhesive because it shrinks and delaminates then it lets moisture get between the fiberglass and the wood substrates. Because the fiberglass is structural to the epoxy coating rather than the part, it’s possible to use a lightweight cloth. Don’t use a cloth a that is too heavy for the intended service, you’ll use a lot more epoxy and have a heavier part, gaining little else. Tests run with Cold Cure epoxy show no appreciable difference in peel strength between the two most popular finishes of fiberglass cloth, Volan and Silane. Four and six ounce cloth are nearly invisible when wet out with clear epoxy resin. Heavier weight cloths begin to show the weave pattern under certain lighting conditions.
Some very porous materials are quite persistent at forming air bubbles. A trick we have used is to heat the whole surface to a temperature about 60°C (140°F). Use a hot air gun or place the wood in the sunlight for awhile. Stop heating and immediately coat the surface. The epoxy will thin on the warm surface and at the same time start to cool it. The air in small pores will begin to contract pulling the thinned epoxy into them. Any air that does rise will be going through thinned epoxy and have an easier time of it.
Avoid using fiberglass mat with epoxy resins. The binder that holds the mat together is designed to be dissolved by the styrene in polyester resins. Most epoxies don’t use styrene as a diluent, making it almost impossible to wet out the mat. Woven roving is wet out well by epoxy although we know of no reason to use it when building a wooden boat.
Cold Cure is an excellent base for varnish. The application of multiple coats of varnish and sanding between coats can be eliminated with NO sanding between coats. The final epoxy coat is sanded to provide a base, then one or two coats of varnish are applied. The result appears to have the depth of ten or
Regardless of the type of the cloth or resin system used, fiberglassing is done essentially the same way. There is no need to be intimidated by fiberglassing, what you are really doing is gluing the cloth to the surface with a minimum amount of resin. Use just enough epoxy to wet out the cloth, you’ll fill the weave of the cloth later with more epoxy.
When this first area has been covered and the cloth has disappeared, take the squeegee and use a fair amount of pressure to squeeze the excess resin away from the wet cloth, working it down into the dry cloth area. This removes excess resin and trapped air, sticking the cloth down right next to the wood surface. The squeegeed cloth should now have a semi-dry look with the weave pattern showing; the cloth itself will be invisible.
Work on as horizontal a surface as possible. Fiberglassing is much easier if you are not fighting gravity.
Keep on going, section by section, until you are finished. If you are working on a very large area use a dry roller cover on the previous three or four sections to give a final smoothing. On smaller boats the roller can be used after the entire hull has been fiberglassed.
The first step in doing a good fiberglass job is to precoat the part. This avoids the problem of having an unsealed porous structure soak up too much epoxy, starving the bond. Precoating doesn’t use any more epoxy than the more difficult one step method (for experienced fiberglasser’s only!) and helps to assure that maximum peel strength is achieved. After the first coat cures fill any holes with an epoxy/microballoon mixture to provide a smooth base for the cloth. Sand lightly but thoroughly to a uniform dull surface. Clean the surface with clean, oil free compressed air or brush off and wipe with a clean damp rag to remove any remaining traces of dust. We do not recommend using acetone or similar solvents for this. Much acetone sold today is reclaimed and may have impurities that interfere with secondary bonding by leaving a film of residue on the surface.
Let the epoxy resin cure to the “green state” stage where it is pliable but no longer tacky unless pressed really hard. Now’s the time to trim the excess cloth. Trim by running a single edged razor blade around where the glass overhangs the edge. Press down any glass that may be lifted from the surface while trimming. The selvege edges of the fiberglass have to be feathered before being covered by another piece of cloth. Wait another hour or so and do the feathering with a Surform. Do it while it is in the right state of cure. Too early and the wet fiberglass will lift, too late and it will be too hard to cut. The alternative is to wait a day or so until it is hard enough to sand.
Next lay the fiberglass out on the precoated, tack free surface, smoothing it out and doing any rough trimming. Masking tape may be necessary to hold the cloth in place if the surface has any slope.
It is not always possible to have a selvage edge on the cloth. Rather than have a cut edge fraying all over the place which can only be cleaned up by a lot of sanding later, here’s a trick that produces a very neat edge. Run a piece of 2” masking tape so that the inner edge of the tape is where you want to stop the glass. Lay down the cloth so that it runs at least an inch past the outer edge of the tape. Wet out the glass past the inner edge and about half way across the tape. When the cure reaches the green state run a single edge razor blade right down the inner edge of the tape. Pull off the tape and presto, you have a nice edge right where you cut the fiberglass. If a little of the cloth lifts, press it back down.
Mix no more than 300 ml of resin and 150 ml of hardener. Work with small batches until you get the hang of it. Start at one end and pour the resin out over an area equal to about 50 ml per square ft. (450 ml does a 1 square meter area). Pour in “S” curves as described in the coating section (on steep surfaces apply the epoxy with a roller cover and roller tray), spreading lightly into the dry areas with a squeegee. We like the rubber squeegee for laying down cloth. Let the resin wet the cloth out. Don’t try to “force” it through the weave with the squeegee. Notice how the cloth disappears as it wets out.
The weave of the cloth can be filled once the resin has reached the green state of cure, preferable the same day. If this is not practical, sand lightly but thoroughly before recoating. Don’t try to sand the weave smooth, fill it with epoxy. Apply fill coats the same as discussed in the preceding section on coating. Several coats may be necessary before the weave is filled. It is possible to thicken the epoxy slightly and do it in one coat using a squeegee. Anti-sag Powder (Cab-O-Sil) works best but don’t use any filler on surfaces that are to be clear finished.
roller cover and a roller pan. Use just enough epoxy to wet out the cloth. When cured finish in the usual way. Corners and edges often require several layers of cloth. Giving thought to a “glassing pattern’ will allow doubling at chines and sheers without going through extra steps. Corners are most easily “patched”. Cut circles of different diameters from cloth scraps. Wet down, dabbing at it with an epoxy soaked brush. Lay down the next larger circle over this wetting it with more epoxy, if necessary. Continue the process until finished. Each larger circle will fray the cut edges of the smaller circle under it. This process is called self-feathering. Use the masking tape trick for the last circle and the job will require little sanding to look nice.
When the weave has been filled the surface should be sanded to prepare it for painting or varnishing. Sand the epoxy, not the fiberglass. Be sure to wear a respirator or dust mask, gloves and a disposable paper suit while sanding. If you do get the fiberglass itch take a cool shower, it will go away in a few hours.
Heavy structural seams are best-done using biaxial tape. Biaxial means that the fibers run at 45 degrees to the way the tape comes off the rolls. When run along a seam ALL the fibers run across the seam at 45 degrees. With regular plain woven tape half the fibers run parallel to the seam and add nothing to strength.
Applying fiberglass overhead is at best a difficult, messy job. Anyone who has tried it once has no desire to repeat the experience and will do everything possible to try to turn the boat over or at least work on a slant. If this is not possible then there are several suggestions for accomplishing this job.
Biaxial tape is heavy at 18 or 24 ounces per square yard and it won’t be clear like lighter tape when wet out with epoxy so don’t use it for bright finished seams. Rather than featheredge biaxial tape by sanding we prefer to fair the edges using an epoxy/ balloon mixture.
If you are working on a relatively small area, wet the surface with mixed resin/hardener and lay a rough cut piece of cloth into the resin. Surface tension will hold it into place without sagging if too much resin is not used. Using a squeegee overhead is a feat no one has yet mastered. Use foam rollers. Once the epoxy has cured you finish the overhead area in the usual manner.
In summary, fiberglassing is a three-step process: 1.
Glassing large overhead areas calls for a different technique and a helper or two. Most successful jobs are done by rolling on a coating, then allowing it to cure to a tacky state. The cloth is then rolled as smoothly as possible onto the tacky coating. This is where you’ll probably need more than one person. Get the wrinkles out as you go along; you won’t be able to slide them out because the tackiness of the coating will hold the cloth in place. Once you’ve got the cloth where you want it press it into the tacky undercoat with a dry foam roller. When it is all smoothed down, wet it out using the
Seal the porous surfaces to prevent starving the joint. Do filling and fairing on the sealed surfaces. Sand lightly but thoroughly.
2. Stick the cloth down leaving a minimum amount of resin in the cloth. 3. Fill the weave any time after the wet cloth has reached the “green stage” and is stuck to the substrate.
Using Fillers with Epoxy Resins
filleting putties to improve tensile strength, and are listed above in descending order of tensile strength improvement.
Cold Cure epoxy properly mixed is intended for both coating and fiberglassing. When used “right out of the jug” the mixture is said to be “unfilled” and it is too thin to be used as a gap-filling adhesive or for fairing and filleting compounds. For these applications certain fillers are added. These materials change the flow and density characteristics of the epoxy system.
Paste pigments (titanium dioxide), black paste (Carbon Black) and aluminum powder are generally used as pigments. Adding white paste pigment produces a white resin coating that is useful for areas where a light color is desired and painting is difficult. Pigments aren’t meant to serve as substitutes for paint in areas exposed to direct sunlight. White paste pigment is useful when added to the final fill coat when fiberglassing, allowing this coat to serve as a cover coat for finish painting.
All powders sold for use with Cold Cure epoxy products are solid materials, falling into four general classes: thixotropic agents, bulking agents, fibers, and pigments. There is some overlapping as to function of certain fillers. For example, plastic minifibers is both fibrous and acts also as a thixotropic agent.
Our pigments are pure dry colorants ground into epoxy resin to produce an epoxy paste pigment. Since they are dispersed into epoxy resin they may be added to the resin side of our epoxy systems to produce a stable pigmented resin. Measure the amount of the pigmented resin used to determine the amount of hardener required. Used in very small amounts these pigments are transparent in an epoxy and can be said to act as dyes. In larger amounts they are opaque.
Anti-sag powder (Zeothix), plastic minifibers and wood flour are thixotropic agents. They turn the epoxy into a thixotropic fluid. Most people are not familiar with the term “thixotropic” though everyone is familiar with the properties of these fluids. They flow under shear stress but do not flow once the stress is removed. Adding these agents to the mixed resin and hardener produces a fluid, which will easily flow under the spreading stress of a putty knife. Once the stress is removed the thickened epoxy retains shape. In short, these powders make the epoxy non-sagging, being added to restrict drainage and make gap filling adhesives.
Fillers change the mechanical properties of the cured resin, however, for all practical purposes these changes can be ignored. Thixotropic agents have the least effect since they are used in the smallest amounts to produce the desired result. Bulking agents reduce tensile strength in proportion to the amount added. Some will initially increase compressive strength. With increasing amounts of additives, though, compressive strength will decrease.
Phenolic microballoons, quartz microspheres, and wood flour are bulking agents. They “bulk out” the epoxy making a lightweight putty-like mix. Although all these thicken the epoxy, only wood flour will make it thixotropic. Attempting to add sufficient microballoon or microspheres a non-sagging fairing putty will result in one that spreads poorly. These materials should be used along with a thixotropic agent. Anti-sag Powder is the best choice because it produces the smoothest compound.
Numerous combinations of filler materials are possible and we have not tested them all. If you have an idea that a certain combination might do something special for you then check it out. Little pieces of scrap plywood are good for this. Think up some destructive tests that will simulate the stresses the material will see in service. Check to see where the failure occurs. If the wood breaks then your combination should work well with wood, at least.
Chopped glass strands, milled glass fibers, and plastic minifibers are fibrous materials that can be incorporated into structural
This is the correct sequence for the addition of filler materials:
wood scarf joints are made at a minimum 8:1 slope. Fillets increase glue surface area and are used to relieve stress concentrations that build at right angle corners. Stringers, for example, should have fillets where they butt onto planking.
Correctly measure and mix resin/ hardener 2. Add fiber fillers, if any and mix well 3. Add bulking agents, if any and mix well 4. Add thixotropic agent and mix well.
Second, make sure that the surfaces being glued are clean, free of grease, oil, wax, and other contaminants that could act as release agents. If the surface is coated with cured epoxy, sand before gluing and wipe the dust off. Remove paint rather than trying to glue onto a painted surface. Epoxy resins stick well to paint although the overall bond strength will be no better than the paint to substrate bond.
Epoxy Resins as Structural Adhesives The mixed viscosity of Cold Cure epoxy is not high enough to make a good gap filling adhesive. Thixotropic agents like Zeothix, Plastic Minifibers, and Wood Flour are used to thicken the epoxy and change the flow characteristics. These fillers will turn the epoxy from translucent to opaque depending on the type and amount used. Anti-sag and Plastic Minifibers make the powder epoxy whitish while Wood Flour turns it reddish-brown. Anti-sag makes a smooth material while epoxy thickened with Plastic Minifibers or Wood Flour will be coarse.
Third, do not overclamp. Epoxy resins require only contact pressure. Overclamping can squeeze most of the adhesive out of the glue joint and the epoxy that is left may be absorbed if the surface is porous, starving the joint. A glue-starved joint is very weak. Use only enough pressure to hold the joint immobile and keep the two surfaces in contact until the epoxy has set – overnight at normal temperatures. Nails, screws, clamps, rubber bands, or staples can all be utilized to do this holding job. Clamp just hard enough to close up the joint.
Microballoons and microspheres should not be routinely used in an adhesive formulation as they reduce tensile strength. Quartz Microspheres may be used as a filler/ thickener for cold molding where the surface area to be bonded is large with respect to the mass. Microspheres are acceptable here because of the large glue surface area involved and the low microsphere loading level.
Fourth, remember that epoxy resins continue to cure and build strength for several days after they solidify. Joints that will be under immediate stress once they are unclamped need more cure time before the clamps are removed. Overnight cures are usually sufficient for most non-stressed joints. A common cause of epoxy joint failures is too much stress before the epoxy has reached sufficient strength. Such a case might occur where a scarfed joint is unclamped and bent into place too soon.
Making an epoxy glue joint is quite simple. First, properly measure and mix the resin and hardener, then coat both mating surfaces with this unfilled epoxy to wet them out. It is not necessary to let this coat cure. Next add the thixotropic agent to the balance of the mixed resin/hardener blend and spread this thickened resin on either of the two surfaces to be glued and close up the joint. That’s all there is to it – but there are some tricks and things to keep in mind.
Fifth, protect any finished wood glue joint from weather degradation. Wood that is allowed to weather will cycle through moisture content extremes. Wood expands as the moisture content increases. This expansion can set up enormous stress concentrations across the glue joint due to uneven rates of expansion on either side of the glue line. These stress concentrations can exceed the strength of any glue, including epoxy resins,
First, remember that the ultimate strength of any glue joint is a function of the glue surface area. The more surface area, the stronger the joint. This is the reason that
causing failure. Protecting the joint by epoxy coating all surfaces of the glued wood stops the moisture cycling and prevents failure because of weathering. This is not a problem for wood glued with epoxy that will not be subject to deep moisture cycling.
Epoxy resins usually bond well with cured thermoset materials like polyester, vinyl ester, and other epoxy resins as long as the cured surface is sanded and wax free. However, you should not try to bond polyester, vinyl ester, or other polymeric materials which are cured with MEKP or other peroxide catalysts to cured epoxy resins.
Cold Cure epoxy works well for use as an adhesive for wood-to-wood and fiberglass cloth-to-wood bonds. When we are asked if it can be used to bond metals and plastics the general answer is that it depends on the materials involved and their intended use.
There are too many materials and combinations to cover every possibility. We suggest that you model any questionable materials that you want to bond. Glue some scraps and test them. Try accelerated aging and retest them. If they survive an hour in 70°C (160°F) water they will probably last for quite a while. You have the ultimate responsibility for your own work.
Metal/metal bonding success depends upon the type of metals bonded, the surface preparation, and the intended service temperature. Generally, we recommend against making structural metal/metal bonds with epoxy resins unless they are specifically formulated for that purpose. Our testing shows that these bonds degrade over time due to different thermal expansion rates setting up shear stress and resultant interfacial failure. For non-structural applications the flexible mastic materials appear to hold better than the more rigid epoxies as they allow for thermal expansion.
Sometimes there’s a need for clear gap filling thickened epoxy. It’s not possible to produce such a material using any of the solid thixotropic agents previously discussed. Our G-1 glue is handy for this since it is clear and thick. 5-Cure is our 1:1 “five minute” epoxy. Items glued with 5-Cure can be stressed in as little as 10 minutes. It is very handy to have in the shop for this reason. Builders often find that “missed screw hole” when ready to lay down the fiberglass cloth. Mix a little 5-Cure, add some Wood Flour or Anti-sag and you’ve got an instant putty to fill the hole. 5-Cure can also be used in combination with Cold Cure as a “spot welder” where clamping is all but impossible.
Metal/wood bonding for non-structural applications may be done successfully with Cold Cure epoxy providing that the metal is clean and bright. Structural applications are best when they are mechanically fastened. Don’t put stainless bolts in epoxy resin. Stainless steel works only in the presence of sufficient oxygen. The epoxy will deprive it of oxygen causing crevice corrosion in the presence of an electrolyte like seawater. Stainless steel fastener failure occurs where the bolt emerges from the epoxy resin.
Coat the pieces to be bonded with thickened Cold Cure epoxy except leave several golf ball-sized bare areas. Mix some 5-Cure and apply to the bare areas. Push the pieces to be bonded together with enough pressure to cause some “ooze out”. Hold in place for about five minutes until the 5-Cure hardens. Now the 5-Cure will hold the pieces together while the Cold Cure epoxy sets.
Bonding to metal alone such as fairings on lead keels will work well with Cold Cure epoxy so long as the lead is bright and free of oxidation. Thermoplastic materials like vinyl, PVC or ABS generally bond poorly with epoxy resins. If you need to bond any of these test them yourself. You will get the best results if you first sand the plastic with coarse paper. Epoxy will not bond to polyethylene, polypropylene, or Teflon. It bonds well to neoprene and polyurethane rubbers.
Unlike our other epoxy systems 5-Cure and 30-Cure, like all similar epoxy products, is water resistant, not waterproof. It is fine for intermittent water contact but should not be constantly immersed.
than sanding the whole fillet down to a common level. Blow or brush off the sanding dust (wear a dust mask!). Make up some more filleting compound and use a broad putty knife to fill the low spots resting the blade against the fillet parallel to the long axis of the filet. Allow the putty to cure and do a final sanding. That’s it! Perfect fillets in two easy steps with little sanding.
Filleting, Fairing, and Molding with Epoxy Resins Cold Cure epoxy is mixed with phenolic microballoons (purple), quartz microspheres (white), or wood flour (brown) to make puttylike material that is used for making cosmetic or structural filleting, fairing, or molding compounds. Rather than supply these compounds in a premixed form, we supply the raw materials so that builders are allowed the versatility of creating customized compounds to fit a specific need.
Before microballoons are painted they should be sealed with epoxy or else the paint goes into the tiny hollows in the broken balloons and the finish will appear ragged. Brush or roll on a coat of epoxy on the sanded balloons, allow to cure and sand lightly before painting.
Filleting is the process of adding an epoxy putty to concave angled corners for cosmetic and structural reasons. Cosmetic fillets are generally “low density” being made by the addition of microballoons which “bulk out” the epoxy. Structural fillets are “high density” and are thickened with anti-sag mini-fibers or wood flour. These fillets sometimes contain glass fiber. Thixotropic agents make the mix non-sagging when sufficient amounts are used. Microballoons and microspheres do thicken the epoxy, but when used in proper loadings do not prevent sagging, and need the addition of a thixotropic agent.
Structural fillets increase the glue joint surface area relieving stress concentration zones that occur at angled corners. They are usually made at the same time that the piece creating the corner is attached. For example, when sheet plywood is glued onto a stringer the excess glue that oozes out can be used to form a fillet. A gloved finger makes a good filleting tool, as these fillets don’t need to be large. Large structural fillets are generally made in a separate operation in a manner similar to making cosmetic fillets. If they aren’t going to show there really is no need to make them pretty. The addition of either milled glass fibers or chopped glass strands improves the tensile strength of structural fillets.
Cosmetic fillets are applied by putting an excess of material along the length of the corner with a putty knife or caulking tube. Be careful not to force big air bubbles into the fillet when putting the putty in the corner. A rounded tool is used to shape the putty by drawing it along the fillet. The sides of the tool should touch both sides of the corner and the tool radius is determined by how rounded the finished fillet will be. Almost any material can be used to make a fillet tool. Plywood paddles work well, are easy to make and are inexpensive. The excess putty will be forced out on either side of the tool where it is scraped off with a putty knife.
Fillets in stitch-and-glue construction usually are fiberglassed. The easiest way to do this is to fiberglass the fillet when it is in a semi-stiff state so that it can still be pushed around with an epoxy-saturated brush. This saves having to sand the fillet after it is cured. Fairing is the operation of filling the low spots to the level of the high spots, eliminating waviness and hollows. The compound used is identical to that of the cosmetic fillet and the operation is similar except that large flat areas are involved. Large drywall broad knives, stiff boards with tapered edged squeegees, and similar tools are useful for fairing. Once the putty has cured it is sanded with large blocks to a level fair with the surrounding area. On very large areas low
Once the fillet is cured it may be sanded. A round edged sanding block with coarse (50 to 60 grit) paper works best. Knock off the high spots with the sandpaper and then come back and fill in the low spots with an additional batch of putty. This is much easier
spots may appear during sanding that will need a second fairing. After final sanding the fairing compound should be sealed with epoxy prior to painting.
months of intense tropical sunlight on horizontal surfaces. Total breakdown will occur about 15 months under these same conditions.
A slick way to fair a large area and avoid a lot of tedious sanding is to use a serrated trowel like the metal one floor tilers use to spread mastic. Apply the fairing putty using this tool leaving a series of parallel ridges that stand proud of the surface. Allow the putty to cure, then sand the area. Notice that all you are sanding is the tops of the ridges – about one fourth of the total surface is being faired. Sanding dust falls into the valleys. Once the ridge tops are fair, the area is cleaned of sanding dust and the valleys are filled with fairing compound using a broad knife with a straight edge. Only a light sanding is then required for final fairing following cure. Seal with epoxy before painting.
Bright finished boats should be finished with a clear coating that contains a UV inhibitor. This inhibitor is sacrificial so the coating must be periodically renewed if the epoxy is to be protected. When the clear coating starts to look dull it’s time to refinish. Old coatings are removed by sanding or are chemically stripped with strong solvents. Test patch an inconspicuous area to make sure that the solvent used does not attack the epoxy base. Solvents and removers containing methylene chloride will etch epoxy surfaces. Don’t use these. Be sure to observe the usual precautions when working with these solvents. Opaque paints do not allow the passage of UV light, offering the best protection of the epoxy coating. A primer coat prior to painting over Industrial Formulators epoxy with these paints is quite helpful for several reasons.
Painting and Finishing Over the years nearly half of the technical service questions we’re asked involve painting and varnishing. More than anything else this has been the area that has caused most people trouble. We have solved these problems by developing our own painting system for epoxy resin surfaces – more on this later.
Besides bottom paint, three broad classes of coatings are commonly used as boat paints. These are the “one part” alkyd and modified alkyd enamels commonly called “oil base paints”, the “two part” epoxy and the two part linear polyurethane (LPU) paints. Since all epoxy based materials eventually chalk in sunlight be careful to consider exposure when using the two-part epoxy paints for exterior finish coats. Two part epoxy primers are recommended as high build sanding base primers for LPU paints.
Industrial Formulators epoxy surfaces may be coated either with opaque paints or finished with clear varnishes. The epoxy surface accepts finishes like any other nonporous surface except that it is chemically active to certain materials because of unreacted amines on the surface and throughout the epoxy matrix.
Be sure that you are getting what you expect when purchasing a marine paint. Paints sold in marine stores today are a triumph of marketing over technology. Remember the adage: “The big print giveth while the small print taketh away.” It is not uncommon to see the pretty face of a paint can staring back at you screaming “Buy me! I am a one part polyurethane”. Yet, when you read the back of the can you find that the ingredients state that it contains polyurethane safflower alkyd resin or some other modified alkyd. If it says alkyd anywhere on the can then it is an alkyd NOT a polyurethane. True polyurethanes often
All outside epoxy surfaces exposed to sunlight must be protected from degradation by ultraviolet (UV) light. This is the invisible short wave length portion of sunlight that causes sunburn. The long-term effect of UV on unprotected epoxy is a dulling of the clear film, followed by chalking and, finally, film cracking and delamination. The initial effects of UV degradation on Industrial Formulators epoxy start after about six
referred to as LPU paints are two parts and cost about two to three times what an alkyd costs. If the ingredients are not specified on the can, then ask for a MSDS on the paint.
“Test patches” are advisable prior to painting or varnishing over an epoxy coating. These test patches will give you a feel for how the various coating materials handle and point out any possible incompatibility problems to their becoming a disaster all over your boat.
Alkyd enamels and related one part solventbased paints and varnishes are easy to work with but may not properly dry on epoxy resins. They may be brushed, rolled or sprayed and dry to a glossy film that is easy to refinish. Their main drawback as a finish is that they are softer than LPU paints and chalk slowly over a period of time.
To do a test patch, coat a small area with the painting system selected to make sure that each paint layer dries properly and adheres well to its substrate. One reason for doing this is that epoxy resins, despite sanding and long cure time remain chemically active to certain components of alkyd paint and varnish systems. Generally, epoxy primers and LPU paints are compatible with epoxy resin coatings and may even chemically bond. However, some of the alkyd enamels and other one part paints and varnishes may not properly dry on epoxy resin coatings. The free unreacted amine in the epoxy resin coating interferes with the action of the mettallic driers in some of these paints. If this happens the paint may surface dry but remain soft and tacky next to the epoxy resin surface.
LPU paints dry very hard with excellent gloss, are not degraded by sunlight and wear very well. Their main drawback is that they require immaculate surface preparation. The solvent based LPU paints contain some very hazardous materials and are difficult to apply. They can turn dull when curing if the humidity is too high. Our experience is that the application of solvent based LPU paints is beyond the skill of most amateur boatbuilders. Because of the ultra high gloss and thin film of LPU paints any imperfection in the substrate will show in the finished coating. Thus, the tendency of the alkyd paints to dull to a semi-gloss finish over time can hide some of the flaws that might otherwise mar an LPU finish. However, if the boat is perfect and you are willing to spend the time and care required to use LPU paints, she’ll even be more beautiful.
A similar chemical phenomenon occurs between the amines in epoxy hardeners and the peroxide catalyst used in polyester and vinyl ester resins and primers. The amines inhibit the action of the peroxide catalyst preventing cure at the interface. For this reason, it is not possible to “gel coat” cured epoxy without specialty barrier coats and it is very risky to use peroxide cured polymers directly over cured epoxy resins. Besides, gel coats don’t look all that good when applied to a male form. Their best use is against a polished female mold.
Use any color you want so long as it is light. If you paint with a dark color and the boat is in the summer sun you are going to experience a number of problems especially if it is a wood boat. First, you’ll get “print through”. This is the telegraphing of the cloth weave pattern to the glossy painted surface. Second, you’ll see what appears to be shrinkage of the epoxy resin (microballoon putty over screw holes, for example). This is caused by the expansion and contraction of the wood fiber due to changing moisture content rapidly aggravated by excess heat soaked up by your darkly painted boat. Finally, the useful life of the boat will be shorter.
Be sure to follow the paint manufacturer’s instructions when doing the test patch. With the exception of the high build two part epoxy primers, all finish paint systems should be applied thinly. Thick coats will not dry properly and may take weeks to “through dry”. Temperature and humidity play an important role in the speed of alkyd paint drying. The higher the temperature and lower the humidity, the faster drying.
You can gauge drying by digging your fingernail into your test patch and scratching. If the paint film is still soft below its surface then it has not finished drying. A dry film is hard all the way through. A simple test called the cross hatch adhesion test will show how the new layer bonds to he substrates. Do this test only on paint that has dried thoroughly. To do this test, take an industrial razor blade and score the surface with a set of 8 parallel lines about an eighth of an inch apart. Score a similar set at 90° degrees from and crossing the first set. The finished lines should look like a giant tic tac toe grid. Take some tan masking tape and press the sticky side into the grid leaving a tail. Press the tape with the back of your fingernail. Grab the tail and jerk the tape off the grid. Examine both the tape and the grid for paint adhesion failures. Except for the grid lines on the tape, no paint should come off on the tape. If it does then you have an adhesion problem and it WILL show up on your boat most likely in the form of paint blisters. Resand with a coarser grit or better, select a different substrate/top coat combination and test it.
Troubleshooting Following are questions we are commonly asked when something goes wrong. We hope that you will read them because if you have a problem the answer may appear below. If it doesn’t then call us on our technical line and we’ll go over it with you. Problem: The epoxy has turned hazy and has white material in the bottom of the jug. Cause and Solution: The epoxy is crystallizing due to storage at too low a temperature. Heat resin to 60°C until crystallization clears. You can do this by placing the material (enclosed in its original container) in a hot water bath or in a black plastic bag in the sun. Problem: The epoxy isn’t curing. Cause and Solution: It was mixed at the wrong ratio. Resin was mixed with resin or vice versa. Remove the uncured material thoroughly by scraping and solvent washing. Mix at proper ratio and reapply.
Once you are satisfied that there are no system compatibility or adhesion problems then you can paint your boat with confidence.
Problem: The epoxy keeps going off in the pot. Cause and Solution: The batch is too big or left too long in the pot. The hardener is too fast for the conditions. Use a smaller batch and get it out of the pot sooner. Change hardeners.
By this time you are probably wondering why we don’t just give you a list of what paint brands you can use. We would if we could but because paint makers are free to modify their formulations without notifying Industrial Formulators we will not recommend a specific brand of paint. The batch we test might have changed by the time information about our results gets to you. It is not possible for us to keep up with all the different brands and lot numbers.
Problem: The epoxy is still gummy. Cause and Solution: The ratio was wrong. It was inadequately mixed. Not enough time has elapsed at the curing temperature. Make sure that the gumminess is not just the amine blush. Wait and see if the cure proceeds. Apply some heat if possible. If it is still gummy then remove the uncured material thoroughly by scraping and solvent washing. Mix at proper ratio and reapply.
3824 William St. Burnaby, BC Canada, V5C 3H9 Technical Support: (604) 294-5723 FAX: (604) 294-8052 Orders Only: 1-800-778-0833